advertisement

APPLIED PHYSICS LETTERS 87, 112507 共2005兲 Reducing the critical current for short-pulse spin-transfer switching of nanomagnets P. M. Braganca,a兲 I. N. Krivorotov, O. Ozatay, A. G. F. Garcia, N. C. Emley, J. C. Sankey, D. C. Ralph, and R. A. Buhrman Cornell University, Ithaca, New York 14853-2501 共Received 22 April 2005; accepted 25 July 2005; published online 9 September 2005兲 We have fabricated permalloy/copper/permalloy nanopillar spin valves designed to reduce the critical current for spin-transfer switching while maintaining thermal stability of the free layer. Pulsed current amplitudes necessary for switching a 4.5-nm-thick permalloy free layer range from 0.4 mA for a 100 ns pulse to 2 mA for a 1 ns pulse, showing that the magnetization must be overdriven to achieve switching on short time scales. Comparisons to Landau–Lifshitz–Gilbert simulations indicate an effective damping parameter ⬇0.03 and spin-torque efficiencies for parallel-to-antiparallel and antiparallel-to-parallel switching that are more symmetric than predicted by recent theoretical models. © 2005 American Institute of Physics. 关DOI: 10.1063/1.2045552兴 Following the prediction1,2 and demonstration3,4 of the spin-transfer switching effect, the use of a spin-polarized current to reversibly switch the orientation of a thin-film nanomagnet has been considered for future high-speed, nonvolatile nanoscale magnetic memory systems.5 Several advances are needed to move this possibility closer to practical reality, with one being a reduction in the currents 共Ic兲 and the current densities 共Jc兲 required to exert sufficient spin torque for 1 – 10-ns-scale switching. Recent studies6,7 have demonstrated that spin-transfer switching can occur on time scales as short as 100 ps, but this requires currents on the order of 10 mA. In contrast, switching currents on the order of 0.1– 0.2 mA are required for making high-density memory circuits using minimum-area metal–oxide–semiconductor field-effect transistors. Strategies for reducing Ic must be subject to the added constraint that the nanomagnet remains thermally stable, which means that devices must use nanomagnets with an energy barrier to reversal UA共T兲 艌 1.0 eV when operating at room temperature 共RT兲, or an even larger barrier 共⬎1.3 eV兲 for an operating temperature of 100 ° C. One approach is to employ nanomagnets with large shape anisotropy and low saturation magnetization. While further improvements are still needed, here we report results from stable spin-valve nanopillar devices that can be switched on the nanosecond time scale with pulse current amplitudes ⬍1 mA. Calculations of spin-transfer switching predict that Ic for a thin-film nanomagnet should scale as Ic ⬃ M s2V␣, where M s is the nanomagnet’s saturation magnetization, V its volume, and ␣ the Gilbert damping parameter.3,8 This holds if the nanomagnet’s demagnetization field 4 M s Ⰷ 2共Hk + Happlied兲, as is the usual case for such thin-film nanomagnets, where Hk is the in-plane shape anisotropy field. In contrast, UA ⬃ HkM sV, so minimizing Ic without reducing UA requires maximizing Hk while decreasing M s. Since Hk increases with film thickness, one should be able to produce a thermally stable nanomagnet with a low Ic by fabricating a comparatively thick nanomagnet structure with pronounced shape anisotropy from a material with small average M s. a兲 Electronic mail: [email protected] We have used electron-beam lithography to pattern magnetic nanopillar structures with high-aspect-ratio 共3:1兲 elliptical cross sections, employing proximity effect corrections to obtain the desired shape in the exposed pattern. These patterns were ion-beam etched into sputtered multilayer stacks of 共all dimensions in nm兲 120 Cu/20 Py/12 Cu/X Py/2 Cu/30 Au, where Py is permalloy 共Ni81Fe19兲 and the thickness X of the Py free layer is either 4.5 or 7 nm. The devices were contacted as described previously.9 Figure 1共a兲 shows a scanning electron microscope image of an approximately elliptical nanopillar having a 40 nm minor axis and a 3:1 aspect ratio, taken before deposition of the top electrode. Figure 1共b兲 is a cross-sectional schematic of the device. Using a 2 nm cubic cell size chosen for simulation convenience, a three-dimensional 共3D兲 micromagnetic simulation 共3D OOMMF兲10 of a 4-nm-thick film of Py with a perfectly elliptical 40 nm⫻ 120 nm cross section predicts Hk ⬇ 1100 Oe, but this neglects the dipole field from our device’s fixed layer. Including this effect, we obtain Hk ⬇ 900 Oe, and further simulation of a complete nanopillar structure having the nonideal shape shown in Fig. 1共a兲 yields Hk = 785 Oe for the free layer. In comparison, 4.2 K measurements of the free-layer easy-axis coercive fields for devices with similar structure to the one in Fig. 1共a兲 yield an average Hc ⬇ 500 Oe. We attribute the difference between FIG. 1. 共a兲 SEM image of a nanopillar. Patterning with electron-beam lithography produces reproducible approximate ellipses with 40⫻ 120 nm dimensions. 共b兲 Cross-sectional schematic for nanopillar structure with convention for current direction. 共c兲 Minor loop of free layer and 共d兲 spin transfer curve at 293 K, with convention for current shown in 共b兲 for a typical device. 0003-6951/2005/87共11兲/112507/3/$22.50 87, 112507-1 © 2005 American Institute of Physics Downloaded 20 Oct 2006 to 128.84.231.88. Redistribution subject to AIP license or copyright, see http://apl.aip.org/apl/copyright.jsp 112507-2 Appl. Phys. Lett. 87, 112507 共2005兲 Braganca et al. the measured Hc and the simulated Hk to the difference between the 4.2 K saturated magnetization of the simulated ideal Py material 共M s = 880 emu/ cm3兲 and that determined by superconducting quantum interference device magnetometry of a thin Py layer sandwiched between Cu films 共M s = 645 emu/ cm3兲, as well as to thin-film roughness which was not modeled in the OOMMF simulation. Using the measured 4.2 K values we obtain UA共4.2 K兲 = M sHkV / 2 ⬇ 1.7 eV. A typical magnetoresistance field scan of the free layer taken with the fixed-layer magnetization orientation held fixed 共minor loop兲 is shown in Fig. 1共c兲, and in Fig. 1共d兲 we show a spin-transfer scan for the same device. The minor loop was taken at T = 293 K for applied magnetic field excursions about the value that cancels out the average dipole field from the fixed layer and shows transitions that are thermally activated due to the finite value of UA共T兲 / kBT. Here UA共T兲 is smaller than UA共0兲 due to both the T dependence of M s and Hk, and more importantly, nonideal or nonmacrospin pathways for thermally activated reversal. The latter is generally modeled11 by assuming a fictitious applied field He such that UA共T兲 = 关M s共T兲Hk共T兲V / 2兴共1 − He / Hk兲2. Typically He / Hk 艋 0.5 for thin-film nanomagnets.11,12 To determine UA 共293 K兲, we made measurements of the average spin-transfer switching current, 具Ic典, from twenty individual scans. This process was then repeated for several different current sweep rates. The results were analyzed with a Kurkijarvi-type treatment of Neel-Brown thermallyactivated magnetic reversal due to a spin torque.5,12–14 In this model we have 冋 具Ic典 = Ic0 1 − 冋 1 kBT 兩Ic0兩 k BT ln UA 0 UA 兩İ兩 册册 , 共1兲 where Ic0 is the zero temperature critical current, and İ is the current sweep rate. In Fig. 2共a兲, we plot 具Ic典 for a 4.5-nm-thick free layer as a function of İ for transitions in which the free-layer moment is driven from parallel to the fixed-layer moment to antiparallel 共P–AP兲 and vice versa 共AP–P兲. Assuming a fluctuation attempt time 0 = 1 ns,12 we Ic0,P-AP obtain UA,P-AP共293 K兲 = 0.85± 0.03 eV, = 0.42± 0.03 mA and UA,AP-P共293 K兲 = 0.73± 0.01 eV, Ic0,AP-P = 0.39± 0.02 mA. The difference in the two activation energies is qualitatively consistent with OOMMF simulations, which show that the dipole field from the fixed layer has a stronger perturbative effect on the free layer when it is in the AP state than when in the P state. Using the measured 293 K value of M s 共560 emu/ cm3兲, we would expect UA0共293 K兲 = 1.3 eV, so the fitted values correspond to He / Hk ⬇ 0.25. Similar measurements for a 7-nm-thick freelayer sample yielded UA,P-AP共293 K兲 = 2.12± 0.1 eV, Ic0,P-AP = 0.77± 0.01 mA, and UA,AP-P共293 K兲 = 1.92± 0.24 eV, Ic0,AP-P = 0.50± 0.02 mA, showing activation energies close to what would be expected from the difference in thickness between 4.5 and 7 nm. While Ic0 is the minimum current for spin-torque switching in the absence of significant thermal activation, fast switching requires higher currents. In the short-pulse regime, the switching time varies approximately as ⬃ 1 / 共I − Ic0兲, with thermal effects resulting in a statistical distribution about this mean value.8,11 We have measured the switching probability of our nanopillar devices as a function of pulse amplitude I, for pulse widths ranging from 100 to 1 ns. In FIG. 2. 共Color online兲 共a兲 Average switching current vs natural log of current ramp rate for a 4.5 nm Py free layer in the P–AP 共夝兲 and AP–P 共䊏兲 switching directions. Error bars represent dispersion in switching current for 20 current sweeps at a given ramp rate. Lines shown are fits to data with a Kurkijarvi-type model. Switching probabilities vs pulse amplitude and single-domain simulation fits for 共b兲 AP–P and 共c兲 P–AP transitions of a 4.5 nm Py free layer. Pulse widths for each curve from left to right are 100 ns 共⽧兲, 10 ns 共䉱兲, 3 ns 共쎲兲, and 1 ns 共夝兲. Lines drawn are curves through points generated by LLG simulation. 共d兲 Switching probabilities vs pulse amplitude and simulations 共solid lines兲 for AP–P switching of a 0.6 nm CoFe/ 5.5 nm PyCu free layer. All measurements were taken at 293 K. Fig. 2, we show results of both positive 共P–AP兲 and negative 共AP–P兲 current-pulse switching for a 4.5 nm device. I ⬎ 4 – 5 Ic0 is required to obtain a high probability of switching with 1 ns pulses. We use the Landau–Lifshitz–Gilbert 共LLG兲 equation macrospin model of the nanomagnet, as modified to include the spin-torque effect,1,11 to simulate the distribution of short-pulse switching probabilities. This equation can be written as: dM̂ ជ +H ជ 兲 − ␥␣ M̂ ⫻ 关M̂ ⫻ 共H ជ +H ជ 兲兴 = ␥ M̂ ⫻ 共H eff lang eff lang dt − I␥បg共兲 共M̂ ⫻ M̂ fixed ⫻ M̂兲, eM sV sin共兲 共2兲 where M̂ and M̂ fixed are unit vectors in the direction of the free- and fixed-layer magnetizations, respectively, ␥ is the gyromagnetic ratio, I is electric current, e is electric charge, ␣ is the Gilbert damping parameter, and Heff is the sum of contributions from the anisotropy, applied, and demagnetization fields. Hlang is a random Langevin field simulating temperature effects, with components determined using a Gaussian with zero mean and a standard deviation fixed by ␣ and T.11,15 The function g共兲 characterizes the strength of the spin torque exerted on the free-layer nanomagnet as a function of the angle between its moment and that of the fixed layer. We assume that g共兲 = A sin共兲 / 关1 + B cos共兲兴, where A and B are constants. The strength of the switching torque is determined by the slopes 兩dg共兲 / d兩 = g0⬘ or g⬘ at the mean starting angles 共0 for P–AP, for AP–P兲, where g0⬘ = A / 共1 + B兲 and g⬘ = A / 共1 − B兲. In simulating the data, we use the activation energies for magnetic reversal obtained from the slow ramp rate measurements to determine the thermal distribution of the angle 0 at the initiation of the pulse. We then Downloaded 20 Oct 2006 to 128.84.231.88. Redistribution subject to AIP license or copyright, see http://apl.aip.org/apl/copyright.jsp 112507-3 Appl. Phys. Lett. 87, 112507 共2005兲 Braganca et al. vary g0⬘, g⬘ , and the Gilbert damping parameter ␣ to obtain fits to the data. Results of the best-fit simulations are also shown in Fig. 2. All three parameters affect the magnitude of current necessary for switching, but ␣ has different consequences than g0⬘ and g⬘ on how the switching probabilities depend on the pulse width, since the influence of Hlang, which depends on ␣, changes between smaller 共⬃1 ns兲 and larger 共⬃100 ns兲 time scales. Thus, there is a unique combination of g0⬘, g⬘ , and ␣ that gives the best agreement with the entire set of measured probability distributions from 1 to 100 ns. From our fits, we generally find that g0⬘ ⬃ 0.2– 0.3 and g⬘ ⬇ 共1 – 1.3兲g0⬘. Several theoretical predictions for g共兲 have been proposed recently based on different treatments of the effects of nonequilibrium spin populations in the electrodes.16–18 Our finding that g0⬘ ⬇ g⬘ is in conflict with the prediction that g0⬘ Ⰶ g⬘ within some of these models.16,18 Perhaps this is due to Py having a short spin-relaxation length,19 comparable to our free-layer thickness, which should act to reduce nonequilibrium electrode effects. The similar values of g0⬘ and g⬘ reflects that the magnitudes of measured critical currents are surprisingly similar for P–AP and AP–P switching, which is advantageous for practical memory devices. Our fits also yield values for the phenomenological damping parameter, ␣ ⬃ 0.025– 0.035, which are comparable to recent reports,20 but are ⬃4⫻ the damping in bulk Py. This high value could be due to nonequilibrium “spin pumping” effects21,22 and/or spin relaxation arising from defects generated in the nanopillar fabrication process. We have also fabricated nanopillar devices with a CoFe共0.6 nm兲 / Py65Cu35共5.5 nm兲 free layer. For this composite material, 具M s典 = 360 emu/ cm3 at 293 K, and a larger area ellipse 共60 nm⫻ 180 nm兲 was required for thermal stability. Pulse-switching results for one such device are shown in Fig. 2共d兲 along with model fits. The torque parameters for this device, g0⬘ = g⬘ = 0.41, are somewhat larger than is typical for the pure Py devices, presumably due to use of the CoFe cladding layer. However, the damping is also much larger, ␣ ⬇ 0.075. This reduces the advantage of the smaller M s, so that significantly smaller values of Ic are not achieved. In summary, we have fabricated high-aspect-ratio, thermally stable nanopillar spin valves that require comparatively low currents for the short-pulse spin-torque switching of the Py and PyCu free layers. Current amplitudes of approximately 4–5 Ic0, where Ic0 is the T = 0 critical current determined by slow-ramp-rate measurements, are required to ensure switching with 1 ns pulses. Fits to the pulse data using the LLG model indicate a high damping parameter ␣ ⬃ 0.025– 0.035, and that the spin-torque function g共兲 is more symmetric than expected theoretically, with initial slopes g0⬘ ⬇ g⬘ ⬃ 0.2– 0.3. Devices with PyCu–alloy free layers have an even higher ␣ ⬇ 0.075. Achieving still lower Ic0 will require further reductions in the free layer’s magnetic moment, coupled with increases in Hk, increases in g0⬘ and g⬘ , and/or decreases in ␣. Additional methods of increasing switching speed for a fixed-pulsed current amplitude include introducing a nonzero equilibrium angle between the free and fixed layers,14,20 or fabricating devices with two fixed layers, one on either side of the free layer.23,24 An enhancement in Hk would result from eliminating the dipole field on the free layer through the use of a properly designed synthetic antiferromagnetic fixed layer. This research was supported by the National Science Foundation 共NSF兲 through its Nanoscale Science and Engineering Center 共NSEC兲 support of the Center for Nanoscale Systems and by the Army Research Office 共ARO兲. Additional support provided by NSF through use of the National Nanofabrication Infrastructure Network/Cornell Nanoscale Facility 共NNIN/CNF兲 facilities and the facilities of the Cornell Materials Research Science and Engineering Center 共MRSEC兲. J. C. Slonczewski, J. Magn. Magn. Mater. 159, L1 共1996兲. L. Berger, Phys. Rev. B 54, 9353 共1996兲. 3 J. A. Katine, F. J. Albert, R. A. Buhrman, E. B. Myers, and D. C. Ralph, Phys. Rev. Lett. 84, 3149 共2000兲. 4 E. B. Myers, D. C. Ralph, J. A. Katine, R. N. Louie, and R. A. Buhrman, Science 285, 867 共1999兲. 5 F. J. Albert, N. C. Emley, E. B. Myers, D. C. Ralph, and R. A. Buhrman, Phys. Rev. Lett. 89, 226802 共2002兲. 6 S. Kaka, M. R. Pufall, W. H. Rippard, T. J. Silva, S. E. Russek, J. A. Katine, and M. Carey, J. Magn. Magn. Mater. 286, 375 共2005兲. 7 T. Devolder, A. Tulapurkar, K. Yagami, P. Crozat, C. Chappert, A. Fukushima, and Y. Suzuki, J. Magn. Magn. Mater. 286, 77 共2005兲. 8 J. Z. Sun, Phys. Rev. B 62, 570 共2000兲. 9 N. C. Emley, F. J. Albert, E. M. Ryan, I. N. Krivorotov, D. C. Ralph, R. A. Buhrman, J. M. Daughton, and A. Jander, Appl. Phys. Lett. 84, 4257 共2004兲. 10 M. J. Donahue and D. G. Porter, OOMMF User’s Guide, Version 1.0, Technical Report No. NISTIR 6376 共National Institute of Standards and Technology, Gaithersburg, MD, 1999兲. 11 R. H. Koch, J. A. Katine, and J. Z. Sun, Phys. Rev. Lett. 92, 088302 共2004兲. 12 I. N. Krivorotov, N. C. Emley, A. G. F. Garcia, J. C. Sankey, S. I. Kiselev, D. C. Ralph, and R. A. Buhrman, Phys. Rev. Lett. 93, 166603 共2004兲. 13 J. Kurkijarvi, Phys. Rev. B 6, 832 共1972兲. 14 E. B. Myers, F. J. Albert, J. C. Sankey, E. Bonet, R. A. Buhrman, and D. C. Ralph, Phys. Rev. Lett. 89, 196801 共2002兲. 15 J. C. Sankey, I. N. Krivorotov, S. I. Kiselev, P. M. Braganca, N. C. Emley, R. A. Buhrman, and D. C. Ralph, cond-mat/0505733. 16 J. Xiao, A. Zangwill, and M. D. Stiles, Phys. Rev. B 70, 172405 共2004兲. 17 J. Manschot, A. Brataas, and G. E. W. Bauer, Appl. Phys. Lett. 85, 3250 共2004兲. 18 J. C. Slonczewski, J. Magn. Magn. Mater. 247, 324 共2002兲. 19 S. D. Steenwyk, S. Y. Hsu, R. Loloee, J. Bass, and W. P. Pratt, J. Magn. Magn. Mater. 170, L1 共1997兲. 20 I. N. Krivorotov, N. C. Emley, J. C. Sankey, S. I. Kiselev, D. C. Ralph, and R. A. Buhrman, Science 307, 228 共2005兲. 21 Y. Tserkovnyak, A. Brataas, and G. E. W. Bauer, Phys. Rev. B 67, 140404 共2003兲. 22 B. Heinrich, Y. Tserkovnyak, G. Woltersdorf, A. Brataas, R. Urban, and G. E. W. Bauer, Phys. Rev. Lett. 90, 187601 共2003兲. 23 L. Berger, J. Appl. Phys. 93, 7693 共2003兲. 24 G. D. Fuchs, I. N. Krivorotov, P. M. Braganca, N. C. Emley, A. G. F. Garcia, D. C. Ralph, and R. A. Buhrman, Appl. Phys. Lett. 86, 152509 共2005兲. 1 2 Downloaded 20 Oct 2006 to 128.84.231.88. Redistribution subject to AIP license or copyright, see http://apl.aip.org/apl/copyright.jsp